c45 according to en 10083 1Origin: bbn STEEL
Thickness: 6mm to 350mm
Length: 200mm to 18000mm
Payment terms: L/C, T/T
Commitment: If we have no the size in stock, it takes about 20 days for us to produce the c45 according to en 10083 1 for you if the quantity can be more than 10 tons.
Describe:Hot rolled steel strip with JIS standard SPHC - shenda-steel…Hot rolled steel strip with JIS standard SPHC,US $ 310 - 490 / Metric Ton, AISI, ASTM, BS, DIN, GBInquiry (Leave message and get the latest price)
c45 according to en 10083 1 Equivalent
C45 EN 10083-2 (Euronorm) - MetalData.InfoC45 EN 10083-2 (Euronorm) Reduction of area: > 40 % Diameter: > 40 mm ; Yield Strength: > 370 MPa Tensile Strength: 630 - 780 MPa Elongation: > 17 % Reduction of area: > 45 % Flat products Thickness: < 8 mm ; Yield Strength: > 490 MPa Tensile Strength: 700 - 850 MPa Elongation: > 14 % Reduction of area: > 35 % Thickness: 8 - 20 mm ; Yield Strength: > 430 MPaEN 10083 C45 steel plate - BEBON INTERNATIONALC45 steel plate is one mainly of high carbon steel, EN 10083 C45 steel plate is for quenching and tempering. Technical delivery conditions for non alloy steels ,these steels are for general engineering purposes C45 EN 10083-2 Number:1.0503 Comparision of steel grades JIS G 4051 S 45 C DIN 17200 C 45 NFA 33-101 AF65-C 45 UNI 7846 C 45 BS 970 070 , c45 according to en 10083 1
Material specification sheet Saarstahl - C45 Material No.: 1.0503 Former brand name: AFNOR: International steel grades: BS: C45, 50CS, 080M46 C45, AF65C45, 1C45 SAE: 1045 Material group: Steel for quenching and tempering according to DIN EN 10083 C Si Mn P S Cr Mo NiSteels for quenching and temperingEN 10083-1:2006 (E) 3 Foreword This document (EN 10083-1:2006) has been prepared by Technical Committee ECISS/TC 23 Steels for heat treatment, alloy steels and free-cutting steels - Qualities and dimensions , the secretariat of which is held byEN 10083 - Otai Special Steel
forgings (see NOTE 2 in EN 10083-1:2006, Clause 1), manufactured from the direct hardening alloy steels for quenching and tempering and the alloy flame and induction hardening steels and supplied in one of the heat treatment conditions given for the different types ofSteel Grade Equivalent Table (EN, SAE/AISI, UNS, DIN, BS , c45 according to en 10083 1Steel Grade Equivalent Table (EN, SAE/AISI, UNS, DIN, BS, UNI, JIS) The table below compares common grades of materials from various international specifications. Note that materials compared are the nearest available grade and may have slight variations in actual chemistry.C45 / 1.0503 - SteelNumber - Chemical composition , c45 according to en 10083 1C45 ( 1.0503 ) EN 10277-2: 2008 Bright steel products. Technical delivery conditions. EN 10083-2: 2006 Steels for quenching and tempering. EN 10250-2: 2000 Open steel die forgings for general engineering purposes. Cr + Mo + Ni = max 0.63 Weldability: Due to the medium-high carbon content it
EN 10083 C45 steel plate - BEBON INTERNATIONALC45 steel plate is one mainly of high carbon steel, EN 10083 C45 steel plate is for quenching and tempering. Technical delivery conditions for non alloy steels ,these steels are EN 1.0503 Material C45 Steel Equivalent, Properties , c45 according to en 10083 1
Grouping system of steel according to TR / ISO 15608. Sub- Group number group number Examples of steel designation Grade , c45 according to en 10083 1 EN 10219-1 EN 10222-4 EN 10248-1 , c45 according to en 10083 1 11.2 C'40, C45 EN 10083-2 EN 10083-2 l) In accordance with the specification of the steel product standards, Re Designation systems for steels - Part 1: Steel namesEN 10027-1:2005 (E) 6 4.3.2 For steels specified in CEN member's national standards and for other steels, steel names shall be allocated by or under the responsibility of the C45 Round Bar, AISI 1045, DIN 1.1191, JIS S45C - Otai , c45 according to en 10083 17. Hardening of DIN C45 Steel Hardening. Harden from a temperature of 820-860oC followed by water or oil quenching. Heat to 820 oC 850 oC hold until temperature is uniform throughout the section, soak for 10 15 minutes per 25mm of section, and quench in water or brine. Or, Heat to 830 oC 860 oC soak as above and quench in oil.Temper immediately while still hand warm.
Drawn Round Steel Barsen 10083-2/06 (c35, c40, c45, c55, c60) DESCRIPTION AND APPLICATIONS Base and non-alloy steel quality suitable for construction of structural elements, as welded, bolted, riveted structures for room temperature applications.Quenched and tempered steels - Salzgitter Flachstahl GmbHThe provisions of EN 10083-2, chapters 5.1.3 and 6 shall apply for delivery and inspection. All quenched and tempered steels are delivered in a hot-rolled and untreated condition. Certificates according to DIN EN 10204 can be supplied as follows: IT, DUN, FAX, e-mail, paper.